## High-pressure  synthesis  and  spin  glass  behavior  of  a Mn/Ir disordered quadruple perovskite CaCu3Mn2Ir2O12

Xubin Ye 1,2 ,  Zhehong Liu 1,2 , Weipeng Wang 1,2 , Zhiwei Hu , Hong-Ji Lin , Shih-Chang Weng , 3 4 4 Chien-Te Chen 4 , Richeng Yu 1,2 , Liu-Hao Tjeng , Youwen Long 3 1,2,5

1 Beijing  National  Laboratory  for  Condensed  Matter  Physics,  Institute  of  Physics, Chinese Academy of Sciences, Beijing 100190, China

2 School of Physical  Sciences,  University  of  Chinese  Academy  of  Sciences,  Beijing 100049, China

3 Max Planck Institute for Chemical Physics of Solids, Dresden 01187, Germany

- 4 National Synchrotron Radiation Research Center, Hsinchu 30076, Taiwan, ROC

5 Songshan Lake Materials Laboratory, Dongguan, Guangdong 523808, China

E-mail: ywlong@iphy.ac.cn

## Abstract

A new 3 d -5 d hybridized quadruple perovskite oxide, CaCu3Mn2Ir2O12, was synthesized by  high-pressure  and  high-temperature  methods.  The  Rietveld  structure  analysis reveals that the compound crystallizes in an AA B  3 4O12-type perovskite structure with space group Im -3, where the Ca and Cu are 1:3 ordered at fixed atomic positions. At the B site the 3 d Mn and the 5 d Ir ions are disorderly distributed due to a rare equal +4 charge states for both of them as determined by X-ray absorption spectroscopy. The competing antiferromagnetic and ferromagnetic interactions among Cu 2+ ,  Mn 4+ ,  and Ir 4+ ions  give  rise  to  spin  glass  behavior,  which  follows  a  conventional  dynamical slowing down model.

Keywords: high-pressure synthesis, quadruple perovskite oxide, spin glass

## 1. Introduction

The  compounds  with AB O3  perovskite  structure  composed  of  a  3D  framework  of corner-sharing B O6 octahedra have attracted much attention, due to their large varieties of physical and chemical properties [1-5]. Chemical substitution either at A or B site is an effective method to tune the structure and physical properties of perovskites. For example, the A -site alkaline earth substitution for rare earth in manganates La1x Ax MnO3 leads  to  insulator-to-metal  and  paramagnetism-to-ferromagnetism  transitions  [6-8]. The B -site  substitution of Fe 4+ by  Co 4+ in  SrFe1x Co O3 causes a series of magnetic x transitions [9]. Specifically, as the x increases, the magnetic ground state changes from helimagnetic antiferromagnetic (AFM) state through cluster glass to ferromagnetic (FM) state with a high Curie temperature. In particular, if three quarters of A site in a simple AB O3 is  substituted  by  a  transition  metal  ion A  ,  one  may  obtain  an  A-site  ordered quadruple perovskite with the chemical formula of AA B  3 4O12 [10-14]. Since the ionic size of a transition metal is much less than that of a typical A -site cation such as alkaline, alkaline earth or rare earth metal, to sustain the perovskite structure, square-coordinated A  O4 units and heavily tilted B O6 octahedra show up in AA B  3 4O12, as presented in figure 1(a). The peculiar coordination environment of A  site is favorable to accommodate a Jahn-Teller distortion ion like Mn 3+ or Cu 2+ . As a Cu 2+ ion with 3 d 9 configuration is concerned, this square coordination may result in a dxy hole state with the Cu-O square planar oxygen bond pointing between x and y [15]. The electronic states of Cu 2+ can exhibit either localized or itinerant behavior depending on the electronic properties of the B -site ions. Moreover, the A  -site Cu 2+ spins can form a magnetic lattice with face-

centered  cubic  symmetry.  The  direct-exchange  interactions  between  the  nearest neighboring Cu 2+ ions compete with the superexchange interactions caused by Cu-OB pathways, leading to unusual magnetic instability and even a magnetic tri-critical point [16-18].

CaCu3Mn4O12  and  CaCu3Ir4O12  are  two  interesting  examples  in A -site  ordered quadruple perovskite family. The former shows a large low-field magnetoresistance response with the absence of Mn 3+ -O-Mn 4+  double-exchange interactions, since only a single Mn 4+ valence state occurs at the B site [19]. The later displays heavy Fermion behavior since the dxy orbital of the Cu 2+ strongly hybridizes with the Ir 5 d orbitals via the Op orbitals, so that the local moments of the Cu are incorporated in the itinerant 5   electrons  of  the  Ir  [20].  This  coupling  leads  to  the  disappearance  of  long-range d magnetic ordering of Cu 2+ ions and strongly enhanced electronic specific heat. Recently, a few AA B B  3 2  2O12-type quadruple perovskites with orderly distributed 3 d /5 d transition metals at the B B /  sites have been discovered [21-23]. One finds that the introduction of 5 d electrons can significantly change the magnetic and electrical transport properties. On account of the interesting properties of CaCu3Mn4O12 and CaCu3Ir4O12, in this study, we prepare a 3 d -Mn and 5 d -Ir hybridized quadruple perovskite oxide CaCu3Mn2Ir2O12 (CCMIO) by using high pressure and high temperature conditions. The crystal structure, charge state, magnetism and electrical transport properties are studied in detail.

## 2. Experiment details

The compound of CaCu3Mn2Ir2O12 was synthesized as black polycrystalline powders.

Highly pure (&gt; 99.9%) CaO, CuO, MnO and Ir powders with a 1:3:2:2 mole ratio were used as starting materials, and excess KClO4 was applied as an oxidizing agent. These reagents were thoroughly mixed in an agate mortar within an argon-filled glovebox, and  then  sealed  into  a  platinum  capsule  with  4.0  mm  in  diameter  and  length.  The capsule was treated at 5.5 GPa and 1673-1773 K for 60 min on a cubic anvil-type highpressure apparatus. The sample was quenched to room temperature (RT) once the heat treatment was finished, and then the pressure was gradually released. The product was washed using deionized water to exclude the residual KCl. In addition, CaCu3Ti4O12 was prepared as described in ref. [24], and Cu2O single crystal was purchased from MaTeck-Material-Tenchnologie &amp; Kristalle GmbH. These two oxides were used as Xray absorption references.

The sample quality and crystal structure were identified by powder X-ray diffraction (XRD) on a Huber diffractometer with Cu K α1 radiation (λ = 1.5406 Å). The diffraction angle  (2θ)  varies  from  10  to  100°with  0.005°   per  step.  The  selected  area  electron diffraction (SAED) was performed at RT along [110] zone axis by a Philips-CM200 transmission electron microscope with a field emission gun operated at 200 keV. The structure refinement was performed by the Rietveld method using the GSAS program [25]. Soft X-ray absorption spectroscopy (XAS) measurements of CuL 2,3 and MnL 2,3 edges  were  carried  out  at  beamline  BL11A  of  the  National  Synchrotron  Radiation Research Center (NSRRC) in Taiwan using the total electron yield mode. The IrL 3 spectra were measured at beamline BL07A of the NSRRC in transmission geometry. The field dependence of the isothermal magnetization ( M ) and temperature-dependent

dc magnetic susceptibility (χdc) were measured using a commercial superconducting quantum interference device magnetometer (MPMS3,  Quantum  Design). The temperature dependence of the ac magnetization ( M  )  and  electrical  transport  were measured on a physical property measurement system (PPMS7, Quantum Design).

## 3. Results and discussions

The crystal structure of CCMIO is characterized by powder XRD at room temperature.

Figure  1(b)  shows  the  XRD  pattern  as  well  as  the  structure  refinement  result.  The Rietveld  analysis  shows  that  the  compound  possesses  an A -site  ordered  perovskite structure with space group Im -3. It means that the Ca and Cu are 1:3 ordered at the A and A  sites, respectively, whereas the Mn and Ir are randomly distributed at the B site. To confirm the Mn/Ir disorder, the SAED pattern was measured along with the [110] zone axis. As shown in the inset of figure 1(b), one cannot find any diffraction spots with h + k + l = odd such as the (111) and (311) spots, revealing the absence of Mn/Ir long-range order at the B site, in agreement with the XRD result. The refined structure parameters are listed in Table 1. In comparison, the lattice parameter of CCMIO (7.4106 Å) is located between those of CaCu3Ir4O12 (7.4738 Å) [20] and CaCu3Mn4O12 (7.2410 Å) [19], suggesting that the Mn and Ir form a solid solution. According to the refined Cu-O bond length, the bond valence sum (BVS) calculations show the valence state of Cu to be +2.09, indicating the presence of a Cu 2+ state with square-planar coordination. Because of the random Mn/Ir arrangement, we cannot obtain the valence states for these two transition metals by BVS calculations.

The oxidation states of the Cu, Mn and Ir ions in CCMIO were investigated by Xray absorption at the CuL 2,3 , MnL 2,3 and IrL 3 edges, respectively. Figure 2(a) shows the CuL 2,3 XAS of CCMIO together with those of Cu2O as a Cu + (3 d 10 ) reference [26] and CaCu3Ti4O12 as a Cu 2+ (3 d 9 )  reference [27] in a quadruple perovskite structure. Typically, for a 3 d 9 Cu 2+ charge state, a strong absorption peak appears around 930.0 eV due to the d 9 → cd 10 transition  [26],  where c indicates  a  hole  in  the  Cu  2 p core. Obviously, the CuL 2,3 spectrum of CCMIO exhibits a very strong single peak at the same energy position as that of CaCu3Ti4O12 revealing the formation of a Cu 2+ valence state in CCMIO with a Cu 2+ O4 square-planar local environment. In comparison, the main peak of Cu2O is shifted to higher energy by about 2.5 eV corresponding to a d 10 → cd 10 s 1 transition [26] of the fully occupied 3 d 10 configuration in Cu . This does + not occur in CCMIO, thus excluding the Cu  state. Figure 2(b) shows the Mn-+ L 2,3 XAS spectra  of  CCMIO  with  those  of  the  reference  oxides  including  the  tetravalent La2MnCoO6 (Mn 4+ , from ref. 28) and the trivalent LaMnO3 (Mn 3+ , from ref. 28) with similar MnO6 octahedral coordination. Compared with LaMnO3, the main absorption peaks of CCMIO move towards higher energy by more than 1 eV. They have however the same energy position and similar spectral features as those of the Mn 4+ reference La2MnCoO6. This finding indicates the presence of a Mn 4+ (3 d 3 ) state in CCMIO. The difference at the shoulder of the Mn L 3 peak might be due to the slightly different charge transfer and ligand field effects between La2MnCoO6 and CCMIO. The observed Mn 4+ state in CCMIO is surprising considering the Mn 3+ state in the Sr3Ru2-xMnxO7 [29].

The IrL 3 XAS spectra of CCMIO, La2CoIrO6 as an Ir 4+ reference (from ref. 30) and

Sr2FeIrO6 as an  Ir 5+ reference  (from  ref.  31)  are  shown  in  figure  2(c).  The  IrL 3  of CCMIO is shifted  by  more  than  1  eV  to  lower  energy  with  respect  to  that  of  Ir 5+ reference  Sr2FeIrO6,  but  locates  at  the  same  energy  as  that  of  the  Ir 4+ reference La2CoIrO6  indicating  the  formation  of  Ir 4+ valence  state. Therefore,  the  XAS measurements confirm the charge combination to be CaCu 2+ 3Mn 4+ 2Ir 4+ 2O12. Usually, for  two cations to form an ordered distribution in a perovskite structure, the charge difference between them is not less than two [32]. The identical charge states between Mn and Ir therefore explains the B-site disorder in CCMIO.  In particular, for most quadruple perovskite oxides with hybridized 3 d -5 d elements at the B site, the 3 d -5 d charge discrepancy is larger than two and then they form an ordered distribution, as exampled by CaCu3Fe2Re2O12, CaCu3Fe2Os2O12, and NaCu3Fe2Os2O12 [21, 22, 33]. The current CCMIO therefore provides an exception where the 3 d and 5 d elements have exactly the same charge state.

The magnetism of CCMIO was studied by both dc and ac magnetizations. Figure 3(a) shows the temperature dependence of zero-field-cooling (ZFC) and field-cooling (FC) dc magnetic susceptibility curves measured at different fields. The ZFC and FC curves separate from each other at a critical temperature T SG  49 K at 0.01 T. Moreover, the T SG systematically shifts towards lower temperatures with increasing magnetic field, accompanied by a gradual reduction in the intensity of  dc and a broadening of the cusp around T SG. These features are indicative of a spin glass transition. Figure 3(b) shows the field-dependent magnetization curves measured at different temperatures. At higher temperatures like 200 K, the linear magnetization behavior is observed, as expected for the  paramagnetism.  At  100  K,  the  magnetization  slightly  deviates  from  the  linear

dependence on field. It may suggest the formation of some short-range FM interactions. At 2 K, one can find remarkable magnetic hysteresis with a ~2 T coercive field, but the magnetization is still not saturated with fields up to 7 T. These observations are in good agreement with the occurrence of spin glass. Above 240 K, the susceptibility data can be fitted using the modified Curie-Weiss (CW) law χ(T) = χ0 + C T /( -θw), where χ0 is the temperature  independent  term  containing  the  core  diamagnetism  and  Van  Vleck paramagnetism. The inset of figure 3(a) shows the fitting results, which give a Curie constant C =  4.75  emu· · ol K m -1 · Oe -1 ,  a  Weiss  temperature  θw  =  58.5  K,  and  a  χ0  = 3.5× 10 -3 emu· mol -1 · Oe -1 .  According  to  the  Curie  constant,  the  effective  magnetic moment is calculated to be μ eff = (8 C ) 1/2 = 6.17 μ B/f.u. If one only considers the spinonly contribution of Cu 2+ and Mn 4+ ions, the effective moment in theory is 6.24 μ B/f.u., which is very close to the fitting one. Therefore, compared to the 3 d Cu 2+ and Mn 4+ , the 5d Ir 4+ may play a minor role on the magnetism of CCMIO. Actually, there is no longrange magnetic order occurring in the isostructural compound CaCu3Ir4O12 [20].

To further clarify the spin glass behavior of CCMIO, ac magnetization was measured at different frequencies by spanning several orders in magnitude. As shown in figure 4(a), the ac magnetization shows a cusp at a spin freezing temperature T f . Moreover, with increasing frequency, the cusp shifts toward higher temperatures with a reduction in magnitude. These features provide another convincing evidence for the occurrence of  spin  glass.  We  can  characterize  the  shift  of T f with  frequency  using  a  physical parameter κ = Δ T f /[ T f Δln(ω)], where the spin freezing temperature T f is  determined from the maximum of M  ,  ω  is  the  ac  frequency,  and  Δ T f and  Δln(ω)  represent  the differences for different frequencies. The κ is calculated to be about 0.8(1)× 10 -2 for CCMIO. The value of κ can offer a criterion for distinguishing a spin glass from a super-paramagnet since the later usually has a larger value of κ. For example, κ is 0.28

for  the  typical  super-paramagnet  compound  a-(Ho2O3)  (B2O3)  [34]  and  0.1  for La0.67Sr0.33MnO3 nanoparticles [35]. The smaller κ value of CCMIO indicates that the compound should be a spin glass system rather than a super-paramagnet, as reported in other spin glasses like the magnetic B12 cluster compound HoB22C2N [36]. In addition, the frequency dependence of T f can be described by a conventional dynamical slowing down model for a three dimension spin glass system with the function τ/τ0 = [( T f  T SG)/ T SG] -zv [37]. Here, τf = 1/ω corresponds to the maximum relation time of the system at T f , τ0 is the intrinsic relaxation time, and zv is the dynamic exponent. Figure 3(b) shows the plot of τf vs T f and the fitting result, yielding zv = 7.67 and τ0 = 8.22× 10 -13 s. The fitted value of τ0 is in accordance with the typical values of 10 -11 -10 -13 s obtained for many canonical spin glasses such as CuMn [34] and Eu0.5Sr1.5MnO4 [38].

The spin glass behavior of CCMIO can be attributed to the competing FM and AFM interactions. According to the Goodenough-Kanamori rules [39, 40], for a Mn 4+ ion with 3 d 3 configuration in a perovskite octahedral crystal field, the Mn 4+ -O-Mn 4+  AFM superexchange interaction is expected to occur as observed in CaMnO3 [41]. On the other  hand,  in A -site ordered  perovskites,  the  presence  of  a  net  ferromagnetic component is possible due to the Cu 2+ (  )Mn 4+ (  ) ferrimagnetic coupling, as reported in CaCu3Mn4O12 [19]. In addition, for the 5 d Ir 4+ , the strong spin-orbital coupling splits the t 2g level into a fully occupied j eff = 3/2 band and a singly occupied j eff = 1/2 state, resulting in a total J eff = 1/2 pseudospin state. An AFM interaction is often shown in J eff = 1/2 systems, such as  Sr2IrO4 and  La2CoIrO6 [42, 43]. As for the spin interaction between the B -site Mn 4+ with half-filled t 2g orbitals and Ir 4+ with half-filled j eff = 1/2 band is concerned, it most probably leads to Mn 4+ (  )Ir 4+ (  ) ferrimagnetic correlation as discussed in another 3 d /5 d hybridized system Pb2FeOsO6 [44]. Therefore, a series of complex and competing FM and AFM interactions are responsible for the spin glass

## behavior of CCMIO.

The temperature dependent resistivity and magnetoresistance effects are measured to characterize the electrical transport properties of CCMIO. As shown in Figure 5(a), the resistivity measured at 300 K is only 15.6 mΩ·cm, which is slightly larger than that observed in CaCu3Ir4O12 with metallic conductivity arising from the itinerant electronic behavior  of  Ir 4+ ions.  In  CCMIO,  although  the  resistivity  lightly  increases  with decreasing  temperature,  taking  into  account  the  polycrystalline  nature  where  the extrinsic  grain  boundaries  play  a  role  on  electrical  transport,  the  weak  temperature dependence of resistivity (especially at higher temperatures such as above 100 K) as well as the disordered perovskite structure with itinerant Ir 4+ state may imply a (bad) metallic electrical behavior. As presented in Figure 6(b), CCMIO shows negative MR effects at different temperatures. Lowering temperature can enhance the MR effects. At 10 K and 7 T, the absolute value of MR is about 10.3%, which is considerably less than that observed in the isostructural compound CaCu3Mn4O12 due to the decrease of Mn 4+ component.

## 4. Conclusions

In summary,  an  Ir-containing  quadruple  perovskite  oxide  CaCu3Mn2Ir2O12  was prepared at 5.5 GPa and 1673-1773 K. The Rietveld analysis based on the powder XRD data reveals an A -site ordered perovskite structure with space group Im -3, in which the Mn and Ir ions are disorderly distributed at the B site.  The  valence states and local environment of Cu, Mn and Ir were investigated by XAS techniques, giving Cu 2+ O4 square-planar coordination at the A  site and Mn 4+ /Ir 4+ O6 octahedral coordination at the B site,  resulting  in  the  charge  combination  of  CaCu 2+ 3Mn 4+ 2Ir 4+ 2O12.  In  magnetism, both dc and ac magnetization measurements indicate a spin glass transition around a

spin  freezing  temperature  of  49  K.  Moreover,  the  spin  glass  behavior  can  be  well described by a conventional dynamic slowing down model.  In comparison with the isostructural compound CaCu3Mn4O12, the MR effect of the current CCMIO is reduced considerably owing to the introduction of Ir.

## Acknowledgments

This  work  was  supported  by  the  National  Key  R&amp;D  Program  of  China  (Grant  No. 2018YFA0305700, 2018YFE0103200), the National Natural Science Foundation of China (Grant No. 51772324, 11574378), and the Chinese Academy of Sciences (Grant No.  QYZDB-SSW-SLH013,  GJHZ1773).  The  research  in  Dresden  was  partially supported by the DFG through SFB 1143. We acknowledge the support from the Max Planck-POSTECH-Hsinchu Center for Complex Phase Materials.

## Reference

- [1] Cava R J, Batlogg B, Vandover R B, Murphy D W, Sunshine S, Siegrist T, Remeika J P, Rietman E A, Zahurak S and Espinosa G P 1987 Phys Rev Lett 58 1676-9
- [2] Wang J, Neaton J B, Zheng H, Nagarajan V, Ogale S B, Liu B, Viehland D, Vaithyanathan V, Schlom D G, Waghmare U V, Spaldin N A, Rabe K M, Wuttig M and Ramesh R 2003 Science 299 1719-22
- [3] Kimura T, Goto T, Shintani H, Ishizaka K, Arima T and Tokura Y 2003 Nature 426 55-8
- [4] Salamon M B and Jaime M 2001 Reviews of Modern Physics 73 583-628
- [5] Dagotto E, Hotta T and Moreo A 2001 Physics Reports-Review Section of Physics Letters 344 1-153
- [6] Jin S, Tiefel T H, Mccormack M, Fastnacht R A, Ramesh R and Chen L H 1994 Science 264 413-5
- [7] Mahendiran R, Tiwary S K, Raychaudhuri A K, Ramakrishnan T V, Mahesh R, Rangavittal N and Rao C N R 1996 Physical Review B 53 3348-58
- [8] Millis A J 1996 Physical Review B 53 8434-41
- [9] Long Y W, Kaneko Y, Ishiwata S, Tokunaga Y, Matsuda T, Wadati H, Tanaka Y, Shin S, Tokura Y and Taguchi Y 2012 Physical Review B 86 064436
- [10] Long Y and Shimakawa Y 2010 New Journal of Physics 12 063029
- [11] Long Y-w, Kawakami T, Chen W-t, Saito T, Watanuki T, Nakakura Y, Liu Q-q, Jin C-q and Shimakawa Y 2012 Chemistry of Materials 24 2235-9
- [12] Shimakawa Y 2008 Inorganic Chemistry 47 8562-70
- [13] Yin Y-Y, Wang X, Deng H-S, Zhou L, Dai J-H and Long Y-W 2017 Acta Physica Sinica 66 030201
- [14] Zhou L, Wang X, Zhang H-M, Shen X-D, Dong S and Long Y-W 2018 Acta Physica Sinica 67 157505
- [15] Xiang H, Liu X, Zhao E, Meng J and Wu Z 2007 Physical Review B 76 155103
- [16] Shimakawa Y and Mizumaki M 2014 Journal of Physics-Condensed Matter 26
- [17] Shimakawa Y and Saito T 2012 Physica Status Solidi B-Basic Solid State Physics

## 249 423-34

- [18] Shimakawa Y, Shiraki H and Saito T 2008 J Phys Soc Jpn 77 113702
- [19] Zeng Z, Greenblatt M, Subramanian M A and Croft M 1999 Phys Rev Lett 82 3164-7
- [20] Cheng J G, Zhou J S, Yang Y F, Zhou H D, Matsubayashi K, Uwatoko Y, MacDonald A and Goodenough J B 2013 Phys Rev Lett 111 176403
- [21] Deng H, Liu M, Dai J, Hu Z, Kuo C, Yin Y, Yang J, Wang X, Zhao Q, Xu Y, Fu Z, Cai J, Guo H, Jin K, Pi T, Soo Y, Zhou G, Cheng J, Chen K, Ohresser P, Yang Yf, Jin C, Tjeng L-H and Long Y 2016 Physical Review B 94 024414
- [22] Chen W-t, Mizumaki M, Seki H, Senn M S, Saito T, Kan D, Attfield J P and Shimakawa Y 2014 Nature Communications 5 3909
- [23] Yin Y-Y, Liu M, Dai J-H, Wang X, Zhou L, Cao H, dela Cruz C, Chen C-T, Xu Y, Shen X, Yu R, Antonio Alonso J, Munoz A, Yang Y-F, Jin C, Hu Z and Long Y 2016 Chemistry of Materials 28 8988-96
- [24] Kadyrova N I, Mel'nikova N V, Ustinova I S and Zainulin Y G 2016 Inorganic Materials 52 1051-4
- [25] Larson A C and Dreele R B V 2004 Los Alamos National Laboratory Report LAUR 86-784
- [26] Tjeng L H, Chen C T and Cheong S W 1992 Physical Review B 45 8205-8
- [27] McGuinness C, Downes J E, Sheridan P, Glans P A, Smith K E, Si W and Johnson P D 2005 Physical Review B 71 195111
- [28] Burnus T, Hu Z, Hsieh H H, Joly V L J, Joy P A, Haverkort M W, Wu H, Tanaka A, Lin H J, Chen C T and Tjeng L H 2008 Physical Review B 77 125124
- [29] Hossain M A, Hu Z, Haverkort M W, Burnus T, Chang C F, Klein S, Denlinger J D, Lin H J, Chen C T, Mathieu R, Kaneko Y, Tokura Y, Satow S, Yoshida Y, Takagi H, Tanaka A, Elfimov I S, Sawatzky G A, Tjeng L H and Damascelli A 2008 Phys Rev Lett 101 016404
- [30] Agrestini S, Chen K, Kuo C-Y, Zhao L, Lin H-J, Chen C-T, Rogalev A, Ohresser P, Chan T-S, Weng S-C, Auffermann G, Vö lzke A, Komarek A C, Yamaura K, Haverkort M W, Hu Z and Tjeng L H 2019 Physical Review B in press

- [31] Dai J H, Yin Y Y, Wang X, Shen X D, Liu Z H, Ye X B, Cheng J G, Jin C Q, Zhou G H, Hu Z W, Weng S C, Wan X G and Long Y W 2018 Physical Review B 97 085103
- [32] Vasala S and Karppinen M 2015 Progress in Solid State Chemistry 43 1-36
- [33] Wang X, Liu M, Shen X, Liu Z, Hu Z, Chen K, Ohresser P, Nataf L, Baudelet F, Lin H-J, Chen C-T, Soo Y-L, Yang Y-f, Jin C and Long Y 2019 Inorganic Chemistry 58 320-6
- [34] Mydosh J A 1993 Spin Glasses: An Experimental Introduction (London: Taylor &amp; Francis)
- [35] Rostamnejadi A, Salamati H, Kameli P and Ahmadvand H 2009 Journal of Magnetism and Magnetic Materials 321 3126-31
- [36] Mori T and Mamiya H 2003 Physical Review B 68 214422
- [37] Hohenberg P C and Halperin B I 1977 Reviews of Modern Physics 49 435-79
- [38] Mathieu R, Asamitsu A, Kaneko Y, He J P and Tokura Y 2005 Physical Review B 72 014436
- [39] Goodenough J B 1955 Physical Review 100 564-73
- [40] Kanamori J 1959 J Phys Chem Solids 10 87-98
- [41] Goodenough J B 1967 Physical Review 164 785-9
- [42] Crawford M K, Subramanian M A, Harlow R L, Fernandezbaca J A, Wang Z R and Johnston D C 1994 Physical Review B 49 9198-201
- [43] Lee S, Lee M-C, Ishikawa Y, Miao P, Torii S, Won C J, Lee K D, Hur N, Cho DY and Kamiyama T 2018 Physical Review B 98 104409
- [44] Zhao Q, Liu M, Dai J, Yin Y, Zhou L, Yang J, Hu Z, Agrestini S, Chen K, Pellegrin E, Valvidares M, Nataf L, Baudelet F, Tjeng L H, Yang Y-f, Jin C and Long Y 2016 Inorganic Chemistry 55 9816-21

Table 1. Structure parameters and BVS results of CCMIO refined from XRD pattern at room temperature.

| parameter                   | CCMIO      |
|-----------------------------|------------|
| a (Å)                       | 7.41060(1) |
| O y                         | 0.1732(4)  |
| O z                         | 0.3034(4)  |
| U iso for Ca (100× Å 2 )    | 1.19(9)    |
| U iso for Cu (100× Å 2 )    | 0.47(2)    |
| U iso for Mn/Ir (100× Å 2 ) | 2.45(1)    |
| U iso for O (100× Å 2 )     | 0.72(8)    |
| d Cu-O (× 4)                | 1.94203    |
| d B-O (× 6)                 | 1.97846    |
| ∠ B-O-B                     | 139.0(1)   |
| ∠ Cu-O-B                    | 109.9(1)   |
| BVS (Cu)                    | 2.09       |
| R wp (%)                    | 4.95       |
| R p (%)                     | 3.25       |

a Crystal data: space group Im -3 (No. 204); atomic sites: Ca 2a (0, 0, 0); Cu 6b (0, 0.25, 0.25); B (Mn/Ir) 8c (0.25, 0.25, 0.25); O 24h (0, y , z ). The BVS values ( Vi ) were calculated using the formula Vi = ∑ j Sij , and Sij = exp[( r0 - rij )/0.37]. The value of r0 = 1.679 for Cu and 4 coordinated oxygen atoms were used.

## Figures and figure captions

Figure 1. (a) Crystal structure of A -site ordered quadruple perovskite AA B  3 4O12 with space group Im -3. (b) XRD pattern and Rietveld refinement result for CaCu3Mn2Ir2O12. Observed (black circle), calculated (red line) and difference (dark yellow line) values are shown together with the allowed Bragg reflection (above ticks). The lower ticks present a small amount of impurity phase IrO2 (~4.9 wt%). The inset in panel b shows a SAED pattern along the [110] zone axis.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00239v1-figure-dde1bd3e-9c63-405e-9764-71209b6dfa94.jpg)

Figure 2. XAS of (a) CuL 2,3 edges of CCMIO and the references CaCu3Ti4O12 and Cu2O, and (b) MnL 2,3 edges of CCMIO and the references La2MnCoO6 (LMCO, from ref. 28) and LaMnO3 (from ref. 28), and (c) IrL 3 edges of CCMIO and the references La2CoIr 4+ O6 (from ref. 30) and Sr2FeIr 5+ O6 (from ref. 31).

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00239v1-figure-ec0bade4-2f1e-447c-a442-cd6b61b18a57.jpg)

Figure  3.  (a)  dc  magnetic  susceptibility  of  CCMIO  measured  at  different  magnetic fields. The  inset  shows  the  Curie-Weiss  fitting  in  240-300  K.  (b) Isothermal magnetization measured at selected temperatures.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00239v1-figure-15a94894-4b1a-4599-a857-c6933c3622a6.jpg)

Figure  4.  (a)  Temperature  dependence  of  ac  magnetic  susceptibility  measured  at different frequencies. (b) The fitted results based on the dynamic slowing down model as described in text.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00239v1-figure-1ef1ffcc-0692-4494-a230-c562e680c9aa.jpg)

Figure 5. (a) Temperature dependence of resistivity measured on heating at zero field for CCMIO. (b) Magnetoresistance as a function of magnetic field measured at different temperatures.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00239v1-figure-1bb9de7a-89ac-49c0-bff5-c90c135eac91.jpg)
Xubin Ye Zhehong Liu Weipeng Wang Zhiwei Hu Hong-Ji Lin Shih-Chang Weng Chien-Te Chen Richeng Yu Liu-Hao Tjeng Youwen Long
High-pressure synthesis and spin glass behavior of a Mn/Ir disordered quadruple perovskite CaCu3Mn2Ir2O12
A new 3d-5d hybridized quadruple perovskite oxide, CaCu3Mn2Ir2O12, was
synthesized by high-pressure and high-temperature methods. The Rietveld
structure analysis reveals that the compound crystallizes in an AA'3B4O12-type
perovskite structure with space group Im-3, where the Ca and Cu are 1:3 ordered
at fixed atomic positions. At the B site the 3d Mn and the 5d Ir ions are
disorderly distributed due to a rare equal +4 charge states for both of them as
determined by X-ray absorption spectroscopy. The competing antiferromagnetic
and ferromagnetic interactions among Cu2+, Mn4+, and Ir4+ ions give rise to
spin glass behavior, which follows a conventional dynamical slowing down model.